Physica C 470 (2010) S725–S727
Contents lists available at ScienceDirect
Physica C journal homepage: www.elsevier.com/locate/physc
STM/STS measurements of the layered superconductor b-HfNCl1x Toshikazu Ekino a,*, Akira Sugimoto a, Kazuhiro Shohara a, Shoji Yamanaka b, Alexander M. Gabovich c a
Hiroshima University, Graduate School of Integrated Arts and Sciences, Higashi-Hiroshima 739-8521, Japan Hiroshima University, Graduate School of Engineering, Higashi-Hiroshima 739-8527, Japan c Institute of Physics, National Academy of Sciences, Nauka Ave. 46, Kyiv 03680, Ukraine b
a r t i c l e
i n f o
Article history: Accepted 26 January 2010 Available online 2 February 2010 Keywords: STM/STS Energy gap Break-junction tunneling b-HfNCl1x
a b s t r a c t Scanning tunneling microcopy/spectroscopy (STM/STS) measurements have been carried out on SmSI ðbÞ type HfNCl1x ðx 0:3Þ samples with T c ¼ 24 K. The STM image on the cleaved surface of ab plane at 5 K clearly reveals a triangular arrangement of bright spots. The separation of the nearest-neighbor spots, 0.369 nm, is in agreement with the a lattice parameter. The STS measurements at 5 K reveal almost constant gap values 2D ¼ 20 meV within the area of at least 10 10 nm2 , thus demonstrating a huge ratio 2D=kB T c ¼ 10. This ratio is very similar to that found in high-T c oxide and organic superconductors. Ó 2010 Elsevier B.V. All rights reserved.
2. Results and discussion
High-T c superconductivity of the compound b-HfNCl1x with layered metal–nitrogen structure was discovered by Yamanaka et al.  Superconductivity with T c ¼ 24 K is induced in this compound by electron doping to HfN double honeycomb layers through the de-intercalation of Cl atoms. Band calculations showed that strongly hybridized Hf 5d and N 2p orbitals form the conduction band . Our previous tunneling break-junction studies clariﬁed very large gap ratio 2D=kB T c > 6 , which unambiguously exceeds the BCS weak-coupling ratio 3.52, where 2D is the superconducting energy gap. Such a huge gap ratio is very rare for conventional superconductors , while it is routinely observed in high-T c cuprate or organic superconductors [5,6]. Other features, for example, low carrier density, the semiconductor–metal transition on carrier doping, the quasi-two-dimensional layered crystal structure, etc. are also similar to those of the copper-based oxides . In this paper, we widened the scope of measurements. In particular, scanning tunneling microcopy/spectroscopy (STM/STS) measurements have been carried out to elucidate the interrelationship between local superconducting energy gap magnitudes and atomic lattice structures. Since we have already measured FeOClðaÞ type Ky TiNCl by STM/STS , it seems instructive to investigate the difference and/or similarity of the superconducting electronic properties between b-HfNCl1x with the double honeycomb network and the a-Ky TiNCl with the rectangular one.
The STM/STS measurements were done with the modiﬁed Omicron LT (low temperature) UHV (ultrahigh vacuum) STM system. Just before the measurements, the sample was cleaved at pressure 108 Pa in the LT–UHV preparation chamber, and then it was carefully in situ transferred to the LT–UHV–STM stage. Scanning measurements were done with a PtIr tip. Fig. 1 shows the STM image taken at 5 K on the cleaved ab surface of the b-HfNCl1x sample ðx 0:3Þ. The sample bias was V = 0.2 V and the tunnel current was I = 0.4 nA. A triangular arrangement of bright spots is clearly visible against the weakly inhomogeneous background. These bright spots correspond to a higher altitude of the scanning tip. The total difference in altitude was 0.2 nm. We can always obtain such quality of the surface, which means that the cleaved surface of b-HfNCl1x is clean and stable under the UHV condition in strong contrast to the cleavage in the ambient atmosphere. From the two-dimensional fast Fouriertransform analysis, the separation of the nearest-neighbor spots was found to be 0.369 nm, which corresponds to the a lattice parameter deduced from X-ray diffraction measurements. By considering the atomic arrangement in the conducting double honeycomb metal–nitrogen network on the ab-plane of b-HfNCl1x , we attributed the bright spots to metallic Hf atoms. To investigate the local superconducting-gap-related features on the nanometer scale, we carried out STS measurements at 5 K simultaneously with the STM measurements. The conductance, GðVÞ ¼ dI=dV, map within the area of at least 10 nm 10 nm in the ab plane reveals fairly uniform magnitudes exhibiting almost constant gap-edge peak positions. Fig. 2 shows such a proﬁle of the STS conductance along the distance of 10 nm.
* Corresponding author. Tel.: +81 82 424 6552; fax: +81 82 424 0757. E-mail address: [email protected]
(T. Ekino). 0921-4534/$ - see front matter Ó 2010 Elsevier B.V. All rights reserved. doi:10.1016/j.physc.2010.01.061
T. Ekino et al. / Physica C 470 (2010) S725–S727
Fig. 1. STM image of b-HfNCl1x (V = 0.2 V, I = 0.4 nA, T = 5 K).
Fig. 2. Distance (x) proﬁle of conductance G(V) for b-HfNCl1x at 5 K.
Relatively homogeneous gap structures are observed with slight variations in G(V) magnitudes. In general, G(V) are weakly asymmetric, i.e., the negative-bias (corresponding to electron tunneling from the sample into the tip) backgrounds are somewhat more pronounced than their positive-bias counterparts, and the junction exhibits substantial leakage at zero bias. The gap-edge peaks at V 10 mV are discernible, although smeared. The almost homogeneous conductance proﬁles and gap features are in strong contrast to the case of a-Ky TiNCl , in which a wide gap distribution was observed, as in the case of bismuth high-T c cuprates .
Fig. 3. Comparison of G(V) from STS for b-HfNCl1x (5 K) and that from breakjunction tunnel spectroscopy (BJTS) for b-Li0:48 ðTHFÞz HfNCl (4.2 K).
The gap value of 2D ¼ 20 meV in b-HfNCl1x revealed by the STS measurements presented here is in accord with that obtained in our previous break-junction tunneling studies . In Fig. 3, G(V) for the above described SIN (superconductor–insulator–normal metal) junctions involving b-HfNCl1x is compared with the break-junction SIS (superconductor–insulator–superconductor) G(V) for b-Li0:48 ðTHFÞz HfNClðTHF;C4 H8 OÞ. Since b-Li0:48 ðTHFÞz HfNCl is extremely reactive and it is more difﬁcult to measure its tunnel spectra than those of b-HfNCl1x , the STM/STS measurements were done mainly on b-HfNCl1x . Nevertheless, it is instructive to compare data for both compounds, because the T c ’s of b-Li0:48 ðTHFÞz HfNCl and b-HfNCl1x are quite similar (25 K and 24 K) and other electronic properties are basically the same in spite of the chemical differences. The peak positions on both curves almost coincide after compensatory rescaling between SIN and SIS junctions as is clearly demonstrated in Fig. 3. Hence, the extremely large gap-like features found earlier in break-junction measurements are now conﬁrmed by STS and can be unambiguously identiﬁed with superconducting gaps, inherent to the studied materials. In other words, the gap magnitudes 2D ¼ 20 meV characterize the b-HfNCl1x compound, demonstrating meanwhile a huge ratio 2D=kB T c ¼ 10. This value substantially exceeds the numbers typical for conventional BCS superconductors, and is very similar to gap to T c ratios found for high-T c oxide and organic superconductors. We note that there is no other available gap measurements on b-HfNCl1x , but the speciﬁc heat of an isostructural b-ZrNCl1x shows much smaller ratio . The gaps observed here are so large that cannot be explained even by an extremely strong electron-intermediate boson coupling. Therefore, it is impossible to interpret our results in the framework of the conventional Cooper-pairing picture, without invoking extra so far unknown factors. Acknowledgements This work was supported by a Grant-in-Aid for Scientiﬁc Research (Nos. 19540370, 19105006, 19014016) of Japan Society of Promotion of Science. A.M.G. highly appreciates FY2007 fellowship No. S-07042 granted by the Japan Society for the Promotion of Science as well as the support given in 2009 by the Visitors Program of the Max Planck Institute for the Physics of Complex Systems (Dresden, Germany).
T. Ekino et al. / Physica C 470 (2010) S725–S727
References    
L. Zhu, S. Yamanaka, Chem. Mater. 15 (2003) 1897. C. Felser, R. Seshadri, J. Mater. Chem. 9 (1999) 459. T. Takasaki, T. Ekino, S. Yamanaka, Physica C 445–448 (2006) 77–79. E.L. Wolf, Principles of Electron Tunneling Spectroscopy, Oxford University Press, New York, 1985.  T. Ekino, S. Hashimoto, T. Takasaki, H. Fujii, Phys. Rev. B 64 (2001) 092510.
 T. Arai, K. Ichimura, K. Nomura, S. Takasaki, J. Yamada, S. Nakatsuji, H. Anzai, Phys. Rev. B 63 (2001) 104518.  J.C. Phillips, A. Saxena, A.R. Bishop, Rep. Prog. Phys. 66 (2003) 2111.  A. Sugimoto, K. Shohara, T. Ekino, S. Yamanaka, J. Phys. Conf. Ser. 150 (2009) 052251.  A. Sugimoto, T. Ekino, H. Eisaki, J. Phys. Soc. Jpn. 77 (2008) 043705.  Y. Kasahara, T. Kishiume, T. Takano, K. Kobayashi, E. Matsuoka, H. Onodera, Phys. Rev. Lett. 103 (2009) 077004.